The Ising model—in which degrees of freedom (spins) are binary valued (up/down)—is a cornerstone of statistical physics that shows rich behaviour when spins occupy a highly frustrated lattice such as kagome. Here we show that the layered Ising magnet Dy3Mg2Sb3O14 hosts an emergent order predicted theoretically for individual kagome layers of in-plane Ising spins. Neutron-scattering and bulk thermomagnetic measurements reveal a phase transition at ∼0.3 K from a disordered spin-ice-like regime to an emergent charge ordered state, in which emergent magnetic charge degrees of freedom exhibit three-dimensional order while spins remain partially disordered. Monte Carlo simulations show that an interplay of inter-layer interactions, spin canting and chemical disorder stabilizes this state. Our results establish Dy3Mg2Sb3O14 as a tuneable system to study interacting emergent charges arising from kagome Ising frustration.
The kagome lattice—a two-dimensional (2D) arrangement of corner-sharing triangles—is at the forefront of the search for exotic states generated by magnetic frustration. Such states have been observed experimentally for Heisenberg1,2,3,4 and planar5,6,7 spins. If Ising spins lie within kagome planes and point either towards or away from the centre of each triangle, the potential for emergent behaviour is shown by considering a spin (magnetic dipole) as two separated + and −magnetic charges: the emergent charge of a triangle is defined as the algebraic sum over the three charges it contains (Fig. 1a)8. Ferromagnetic nearest-neighbour interactions favour states, yielding six degenerate states on each triangle. This macroscopic ground-state degeneracy leads to a zero-point entropy S0≈ ln R per mole of Dy (where R is the molar gas constant), and suppresses spin order9, in analogy to three-dimensional (3D) spin-ice materials10,11. The long-range magnetic dipolar interaction generates an effective Coulomb interaction between emergent charges, driving a transition to an emergent charge ordered (ECO) state that is absent for nearest-neighbour interactions alone8,12. In this state, + and − charges alternate, but the remaining threefold degeneracy of spin states for each charge means that spin order is only partial (Fig. 1b). The ECO state has two bulk experimental signatures: non-zero entropy S0≈0.11R per mole of Dy12, and the presence of both Bragg and diffuse magnetic scattering in neutron-scattering measurements13,14. Experimentally, kagome ECO states have been observed in spin-ice materials under applied magnetic field15,16 and nano-fabricated systems in the 2D limit14,17,18,19. However, a crucial experimental observation has remained elusive—namely, observation of the spatial arrangement of emergent charges in a bulk kagome material.
In this article, we show that an ECO state exists at low temperature in the recently-reported bulk kagome magnet Dy3Mg2Sb3O14 (ref. 20). Our experimental evidence derives from neutron-scattering and thermodynamic measurements, while Monte Carlo (MC) simulations reveal that this ECO state is stabilized by a combination of interactions between kagome layers, spin canting out of kagome layers and chemical disorder.
Structural and magnetic characterization
Structural and magnetic characterization suggests that Dy3Mg2Sb3O14 (ref. 20) is an ideal candidate for an ECO state. The material crystallizes in a variant of the pyrochlore structure (space group Rm20) in which kagome planes of magnetic Dy3+ alternate with triangular layers of non-magnetic Mg2+ (Fig. 1c). X-ray and neutron powder diffraction measurements confirm the absence of a structural phase transition to ≲0.2 K (Supplementary Figs 1 and 2 and Supplementary Tables 1 and 2) and reveal a small amount of site disorder in our sample, with 6(2)% of Dy kagome sites occupied by Mg (and 18(6)% of Mg sites occupied by Dy). Curie-Weiss fits to the magnetic susceptibility (Fig. 1d) yield a Curie-Weiss constant θCW=−0.1(2) K for fitting range 5≤T≤50 K, consistent with ref. 20 (however, the value depends strongly on fitting range). Demagnetization effects may also be significant—increasing θCW by 1.4 K in spin-ice materials21—but cannot be quantitatively determined for a powder sample. The local Dy environment in Dy3Mg2Sb3O14 is similar to the cubic spin ice Dy2Ti2O7 (ref. 22) (Supplementary Fig. 3), suggesting that Dy3+ spins have an Ising anisotropy axis directed into or out of the kagome triangles with an additional component perpendicular to the kagome planes. Experimentally, we confirm Ising anisotropy at low temperatures using isothermal magnetization measurements, which are ideally described by paramagnetic Ising spins with magnetic moment μ=10.17(8) μB per Dy (Fig. 1e). Moreover, our inelastic neutron-scattering measurements show that the ground-state Kramers doublet is separated from the first excited crystal-field state by at least 270 K (Supplementary Fig. 4), indicating that crystal-field excitations are negligible at the low temperatures (≤50 K) we consider.
Low-temperature spin correlations
The magnetic specific heat Cm(T) shows that spin correlations start to develop below 5 K and culminate in a large anomaly at T*=0.31(1) K that we attribute to a magnetic phase transition (Fig. 2a and Supplementary Fig. 5). Below 0.20 K, the spins fall out of equilibrium, as is also reported in spin-ice materials23. In zero applied field, the entropy change ΔSm(T) from 0.2 K to T=10 K is slightly less than the expected Rln2 for random Ising spins; however, the full Rln2 entropy is recovered in a small applied field of 0.5 T. The 0.05(3)R difference between ΔSm(10 K) in zero field and in a 0.5 T field could be explained either by ECO (with entropy 0.11R in the 2D case12), or by the ∼6% randomly-oriented orphan Dy spins on the Mg site (with entropy 0.06 Rln2). Neutron-scattering experiments on a powder sample of 162Dy3Mg2Sb3O14 distinguish these two scenarios by revealing the microscopic processes at play across T*. Figure 2b shows magnetic neutron-scattering data at 0.5 K (above T*) and at the nominal base temperature of 0.03 K (below T*). At 0.5 K, our data show magnetic diffuse scattering only, with a broad peak centred at ≈0.65 Å−1 that is characteristic of ice-rule correlations in structurally related pyrochlore magnets24. In contrast, at 0.03 K, strong magnetic diffuse scattering is observed in addition to magnetic Bragg peaks. These peaks develop at T≤0.35 K; that is, as T* is crossed. No additional peaks are observed on further cooling and the magnetic scattering does not change between 0.1 and 0.03 K. Between 0.03 and 50 K, the scattering is purely elastic within our maximum experimental resolution of ≈17 μeV (Supplementary Fig. 6), indicating that the spins fluctuate on a timescale longer than ∼0.2 ns. Our 0.03 K data suggest two immediate conclusions. First, the magnetic Bragg peaks are described by the propagation vector k=0; that is, order preserves the crystallographic unit cell below T*. Second, a large fraction of the magnetic scattering is diffuse; hence, correlated spin disorder persists below T* and involves the majority of spins. These results cannot be explained by only a small fraction of orphan spins, but are consistent with an ECO state13,14.
Average magnetic structure
We use reverse Monte Carlo (RMC) refinement25,26 to fit spin microstates to data collected between 0.03 and 4 K. A single RMC microstate can capture both the average spin structure responsible for Bragg scattering and the local deviations from the average responsible for diffuse scattering (Fig. 2b and Supplementary Fig. 7). We determine the average spin structure by two methods: first, by averaging refined RMC microstates onto a single unit cell; second, by using a combination of symmetry analysis and Rietveld refinement to model the magnetic Bragg profile (obtained as the difference between 0.03 and 0.5 K data) (Fig. 2c). Details of the Rietveld refinements are given in Supplementary Note 1. Both approaches yield the same all-in/all-out average spin structure (inset to Fig. 2c and Supplementary Fig. 8). The ordered magnetic moment at 0.03 K, μavg=2.82(4) μB per Dy, is much less than the total moment of μ≈10 μB. These results are consistent with ECO: Fig. 2d shows that averaging over the three possible ECO microstates for a given triangle generates an all-in/all-out average structure, as observed experimentally; moreover, the expected ordered moment for ECO, μ/3≈3.3 μB per Dy13, is in general agreement with the measured value of 2.82(4) μB per Dy.
Evidence for emergent charge order
To look for signatures of ECO in real space, we compare the temperature evolution of μavg with the percentage of charges (Fig. 3a). The latter quantity, f±3, takes a value of 25% for random spins, 100% for an all-in/all-out microstate, and 0% for a microstate that fully obeys the ice rule. The value of f±3 extracted from RMC refinements decreases with lowering temperature to a minimum value of <5% below 1 K; these values represent upper bounds because RMC refinements were initialized from random microstates. Crucially, below T*, the rule is obeyed while μavg is non-zero (Fig. 3a); this coexistence of ice-rule correlations with an all-in/all-out average structure is a defining feature of the ECO state13,14. We confirm ECO by calculating the charge-correlation function , the average product of charges separated by radial distance rab on the honeycomb lattice formed by the triangle midpoints. At 0.5 K, this function decays with increasing rab, indicating that charges are disordered (Fig. 3b). At 0.03 K, shows two key features that indicate an ECO state: a diverging correlation length, and an alternation in sign with a negative peak at the nearest-neighbour distance (Fig. 3c). The magnitude of found experimentally (≈0.6=(0.94 × 3μavg/μ)2) is smaller than the value of unity corresponding to an ideal ECO state, which indicates that the alternation of charges contains some errors; we show below this is probably due to the presence of site disorder.
Explanation of emergent charge order
Why does Dy3Mg2Sb3O14 show fundamentally the same ECO as predicted for a 2D kagome system of in-plane Ising spins? This is far from obvious, because the real material differs from the existing model8 in three respects: (i) the spins are canted at an angle of 26(2)° to the kagome planes, (ii) the planes are layered in 3D and (iii) there is Dy/Mg site disorder (Fig. 2c). This puzzle is elucidated by Monte Carlo simulations for a minimal model containing the nearest-neighbour exchange interaction J=−3.72 K determined for structurally-related Dy2Ti2O7 (refs 22, 27), and the long-range magnetic dipolar interaction D=1.28 K calculated from experimentally determined Dy–Dy distances. In 2D, spin canting interpolates between two limits—an ECO transition followed by lower-temperature spin ordering for in-plane spins8, and a single spin-ordering transition for spins perpendicular to kagome planes28—and hence destabilizes ECO compared with the 2D in-plane limit. In contrast, the stacking of kagome planes stabilizes 3D ECO—uniquely minimizing the effective Coulomb interaction between emergent charges—but leaves the spin-ordering transition temperature essentially unchanged. The effect of random site disorder is shown in Fig. 3d. Disorder broadens the specific-heat anomalies and suppresses the ECO transition temperature. In spite of this, we find that a distinct ECO phase persists for 6% Mg on the Dy site; that is, the estimated level of disorder present in our sample of Dy3Mg2Sb3O14. Moreover, simulated magnetic specific-heat (Fig. 3d) and powder neutron-scattering (Supplementary Fig. 9) curves with ∼4 to 6% Mg on the Dy site show remarkably good agreement with experimental data, especially given that J is not optimized for Dy3Mg2Sb3O14 .
Implications of emergent charge order
An ECO microstate can be coarse-grained into a magnetization field with two components: the all-in/all-out average spin structure with non-zero divergence, and the local fluctuations from the average that are captured by (divergence-free) dimer configurations on the dual honeycomb lattice13. These two components are independent, which leads to descriptions of the ECO state in terms of spin fragmentation13,14. Without site disorder, the fluctuating component yields pinch-point features in single-crystal diffuse-scattering patterns, the signature of a Coulomb phase13,29. Figure 3e shows that the introduction of site disorder blurs the pinch points and reduces the magnitude of the ordered moment in the ECO phase. We find good overall agreement between patterns from model simulations with ∼4 to 6% Mg on the Dy site and from RMC microstates refined to powder data (Fig. 3e). These results suggest that pinch-point scattering could be observed in single-crystal samples of Dy3Mg2Sb3O14 with low levels of disorder. Our simulations also suggest why a transition from ECO to spin ordering is not observed experimentally: single-spin-flip dynamics (arguably more appropriate to real materials) become frozen in the ECO state and non-local (loop) dynamics are required to observe the spin-ordering transition in Monte Carlo simulations.
The ECO state in Dy3Mg2Sb3O14 is the first realization of ordering of emergent degrees of freedom in a solid-state kagome material. Phase transitions driven by emergent excitations are rare—related examples being the critical end-point in spin ice11,30,31 and the recent report of spin fragmentation in pyrochlore Nd2Zr2O7 (ref. 32). Moreover, the unusually slow spin dynamics offer the exciting possibility of measuring finite-time (Kibble-Zurek) scaling at the ECO critical point31. The ECO state in Dy3Mg2Sb3O14 presents an intriguing comparison with other partially ordered magnets. In Gd2Ti2O7, symmetry breaking yields two inequivalent Gd sites, only one of which orders33,34; in contrast, in the ECO state, all spins possess both ordered and disordered components. In Ho3Ga5O12, local antiferromagnetic correlations coexist with average antiferromagnetic order35, whereas in the ECO state, the average order is antiferromagnetic (all-in/all-out) while the local correlations are ferromagnetic (two-in/one-out or vice versa). Whether the predicted spin-ordering8 eventually occurs in Dy3Mg2Sb3O14 remains to be seen: spin freezing36,37 or site disorder may prevent its onset. We expect physical and/or chemical perturbations to control the properties of Dy3Mg2Sb3O14 ; for example, application of magnetic field slightly tilted from the c-axis should drive a Kastelyn transition towards spin-ordering15,16; modified synthesis conditions may allow the degree of site mixing to be controlled20; and application of chemical pressure may alter the spin-canting angle and/or the distance between kagome layers, potentially generating a novel spin-ordering phase instead of ECO for sufficiently large canting28. Substitution of Dy3+ by other lanthanide ions20,38,39,40 may increase the ratio of exchange to dipolar interactions, offering promising routes towards exotic spin-liquid behaviour: dimensionality reduction by effective layer decoupling (when exchange dominates over dipolar interactions), and realization of quantum kagome systems with local spin anisotropies.
Powder samples of Dy3Mg2Sb3O14 were prepared from a stoichiometric mixture of dysprosium (III) oxide (99.99%, Alfa Aesar*), magnesium oxide (99.998%, Alfa Aesar*) and antimony (V) oxide (99.998%, Alfa Aesar*). For neutron-scattering experiments a ∼5 g sample isotopically enriched with 162Dy (94.4(2)% 162Dy2O3, CK Isotopes*) was prepared. For all samples, starting materials were intimately mixed and pressed into pellets before heating at 1,350 °C for 24 h in air. This heating step was repeated until the amount of impurity phases as determined by X-ray diffraction was no longer reduced on heating. The enriched sample contained impurity phases of MgSb2O6 (6.4(5) wt%) and Dy3SbO7 (0.97(8) wt%), the latter of which orders antiferromagnetically at T≈3 K (ref. 41).
*The name of a commercial product or trade name does not imply endorsement or recommendation by the National Institute of Standards and Technology (NIST).
X-ray diffraction measurements
Powder X-ray diffraction was carried out using a Panalytical Empyrean* diffractometer with Cu Kα radiation (λ=1.5418 Å). Measurements were taken between 5≤2θ≤120° with Δ2θ=0.02°.
*The name of a commercial product or trade name does not imply endorsement or recommendation by NIST.
Powder neutron diffraction measurements were carried out on the General Materials (GEM) diffractometer at the ISIS Neutron and Muon Source, Harwell, UK42, at T=0.50, 0.60, 0.90, 2.0, 4.0, 25 and 300 K. For T=25 and 300 K measurements, around 4.2 g of isotopically enriched powder was loaded into a ϕ=6 mm vanadium can and cooled in a flow cryostat. For measurements at T≤25 K, the same sample was loaded into a ϕ=6 mm vanadium can, which was attached directly to a dilution refrigerator probe and loaded within a flow cryostat. Inelastic neutron-scattering experiments were carried out on the Disk Chopper Spectrometer (DCS) at the NIST Center for Neutron Research, Gaithersburg MD, USA43, at T=0.03, 0.10, 0.20, 0.30, 0.35, and 0.50 K. Around 1.1 g of isotopically enriched powder was loaded into a ϕ=4.7 mm copper can and mounted at the base of a dilution refrigerator. The temperature was measured at the mixing chamber and does not necessarily reflect the sample temperature for 0.1 and 0.03 K, as the spins progressively fall out of equilibrium. On DCS, data were measured with incident wavelengths of 1.8, 5 and 10 Å. The 1.8 Å data were used to look for crystal-field excitations (Supplementary Fig. 4). The 10 Å data were used to look for low-energy quasi-elastic scattering (Supplementary Fig. 6). The 5 Å data were integrated over the energy range −0.15≤E≤0.15 meV to obtain the total scattering (Supplementary Fig. 10). Data reduction was performed using the MANTID and DAVE44 programs. All data were corrected for detector efficiency using a vanadium standard, normalized to beam current (GEM) or incident beam monitor (DCS), and corrected for absorption by the sample.
Combined Rietveld analysis of the 300 K X-ray and neutron (GEM) diffraction data was carried out using the FULLPROF suite of programs45. The individual patterns were weighted so that the total contribution from X-ray and neutron diffraction was equal; that is, data from each of the five detector banks on GEM was assigned 20% of the weighting of the single X-ray pattern. The neutron scattering cross-section for Dy was fixed to bDy=−0.6040, fm, to reflect the isotopic composition as determined by inductively coupled plasma mass spectrometry. Peak shapes were modelled using a pseudo-Voigt function, convoluted with an Ikeda-Carpenter function or an axial divergence asymmetry function for neutron and X-ray data, respectively. Backgrounds were fitted using a Chebyshev polynomial function. At 25 K, Rietveld analysis of only the neutron diffraction data was carried out. In addition to the impurity phases observed in X-ray diffraction, a small amount (<1 wt%) of vanadium (IV) oxide from corrosion of the vanadium sample can was also observed in the neutron-diffraction data. The fit to 300 K data is shown in Supplementary Fig. 1, refined values of structural parameters are given in Supplementary Table 1, and selected bond lengths are given in Supplementary Table 2.
Magnetic susceptibility measurements, χ(T)=M(T)/H, were made using a Quantum Design* Magnetic Properties Measurement System (MPMS) with a superconducting interference device (SQUID) magnetometer. Measurements were made after cooling in zero field (ZFC) and in the measuring field (FC) of μ0H=0.1 T over the temperature range 2≤T≤300 K. Isothermal magnetization M(H) measurements were made using a Quantum Design* Physical Properties Measurement System (PPMS) at selected temperatures 1.6≤T≤80 K between −14≤μ0H≤14 T. A global fit to the M(H) data for T≥5 K (Fig. 1e) was performed using the powder-averaged form for free Ising spins,
where H is applied magnetic field, and magnetic moment μ is the only fitting parameter21. The fitted value μ=10.17(8) μB per Dy is in close agreement with the expected value of 10.0 μB for a Kramers doublet ground state with g=4/3 and mJ=±15/2; in particular, the reduced value of the saturated magnetization, Msat≈μ/2, is as expected for powder-averaged Ising spins21.
*The name of a commercial product or trade name does not imply endorsement or recommendation by NIST.
Heat-capacity measurements were carried out on a Quantum Design* Physical Properties Measurement System instrument using dilution fridge (0.07≤T≤4 K) and standard (1.6≤T≤250 K) probes in a range of measuring fields, 0≤μ0H≤0.5 T. To ensure sample thermalization at low temperatures, measurements were made on pellets of Dy3Mg2Sb3O14 mixed with an equal mass of silver powder, the contribution of which was measured separately and subtracted to obtain Cp. The magnetic specific heat Cm was obtained by subtracting modelled lattice Cl and nuclear Cn contributions from Cp. We obtained Cl by fitting an empirical Debye model to the 10<T<200 K data, with θD=272(13) K. To obtain a lower bound on the contact hyperfine and electronic quadrupolar contributions to Cp23,46, we used previous experimental results on dysprosium gallium garnet47, a related material for which these contributions are known down to T=0.037 K. Correcting for the larger static electronic moment ≈4.2 μB of dysprosium gallium garnet compared with 〈μ〉≥2.5 μB below 0.2 K for Dy3Mg2Sb3O14, we obtained the high-temperature tail of the nuclear hyperfine contributions as Cp=A/T2 with A=0.0032 J K (Supplementary Fig. 5).
*The name of a commercial product or trade name does not imply endorsement or recommendation by NIST.
Average magnetic structure analysis
The magnetic Bragg profile was obtained by subtracting data collected at T<0.5 K from the 0.5 K data. Refinements were carried out using the Rietveld method within the FULLPROF suite of programs45, as described above. For the magnetic-structure refinement shown in Fig. 2c, candidate magnetic structures were determined using symmetry analysis48 via the SARAH49 and ISODISTORT50 programs, as described in Supplementary Note 1. The average magnetic structure is described by the irreducible representation Γ3, in Kovalev’s notation51. The basis vectors of the magnetic structure are given in Supplementary Table 3 and refined values of structural parameters are given in Supplementary Table 4.
Magnetic total scattering
To isolate the total magnetic contribution to the neutron-scattering data, data collected at a high temperature Thigh>>θCW were subtracted from the low-temperature data of interest, where Thigh=25 K (GEM data) or 50 K (DCS data). For the data obtained below the magnetic ordering temperature of the Dy3SbO7 impurity phase (≈3 K (ref. 41)), a refined model of the magnetic Bragg scattering of Dy3SbO7 was subtracted, as described in Supplementary Note 2 (we note that the orthorhombic crystal structure of Dy3SbO7 (ref. 52) allowed the impurity Bragg peaks to be readily distinguished from sample peaks). The fit to neutron data of the Dy3SbO7 magnetic-structure model is shown in Supplementary Fig. 11, the magnetic basis vectors are given in Supplementary Table 5, and refined values of structural parameters are given in Supplementary Table 6. The data were placed on an absolute intensity scale (barn sr−1 Dy−1) by normalization to the calculated nuclear Bragg profile at Thigh.
Reverse Monte Carlo refinements
Refinements to the total (Bragg+diffuse) magnetic scattering were performed using a modified version of the SPINVERT program53 available from J.A.M.P. In these refinements, a microstate was generated as a periodic supercell containing N=7776 Dy3+ spin vectors , where μ=10.0 μB is the fixed magnetic moment length, the unit vector specifies the local Ising axis determined from Rietveld refinement, and the Ising variable σi=±1. A random site-disorder model with 6% non-magnetic Mg on the Dy site was assumed, and Si≡0 for atomic positions occupied by Mg. Ising variables were initially assigned at random, and then refined against experimental data in order to minimize the sum of squared residuals,
where I(Q) is the magnetic total-scattering intensity at Q, subscripts ‘calc’ and ‘expt’ denote calculated and experimental intensities, respectively, σ(Q) is an experimental uncertainty, and W is an empirical weighting factor. For data collected on GEM, a refined flat-in-Q background term was included in the calculated I(Q). For data collected at T≤0.35 K, we obtain Icalc(Q)=IBragg(Q)+Idiffuse(Q)−Irandom(Q), where subscripts ‘Bragg’, ‘diffuse’ and ‘random’ indicate magnetic Bragg, magnetic diffuse and high-temperature contributions, respectively. Here, Irandom(Q)=C[μf(Q)/μB]2, where the constant C=(γnre/2)2=0.07265 barn and f(Q) is the Dy3+ magnetic form factor54. The Bragg and diffuse contributions were separated by applying the identity Si≡〈Si〉+ΔSi to each atomic position55, where the average spin direction 〈Si〉 is obtained by vector averaging the supercell onto a single unit cell, and the local spin fluctuation ΔSi≡Si−〈Si〉. The Bragg contribution is given by
in which G is a reciprocal lattice vector with length G, V is the volume of the unit cell, Nc is number of unit cells in the supercell, R(Q−G) is the resolution function determined from Rietveld refinement56. The magnetic structure factor F⊥(G)=∑i〈Si〉⊥ exp(iG·ri), where supercript ‘⊥’ indicates projection perpendicular to G, and the sum runs over all atomic positions in the unit cell. The diffuse contribution is given by
where sums run over all atomic positions in the supercell, rij is the radial distance between positions i and j, and the correlation coefficients Aij=ΔSi·ΔSj−(ΔSi·rij)(ΔSj·rij)/ and Bij=3(ΔSi·rij)(ΔSj·rij)/−ΔSi·ΔSj (refs 53, 57). For data collected at T≥0.5 K, which show no magnetic Bragg scattering, we obtain Icalc(Q)=Idiffuse(Q)−Irandom(Q), where Si replaces ΔSi everywhere. All refinements employed the Metropolis algorithm with single-spin flip dynamics, and were performed for 200 proposed flips per spin, after which no significant reduction in χ2 was observed. Fits-to-data at T=0.03, 0.20, 0.50, 0.60, 0.90, 2.0 and 4.0 K are shown in Supplementary Fig. 7.
Monte Carlo simulations
Simulations were performed for the dipolar spin ice model27,58, extended to the geometry of interest in this work. The model is defined for Ising spins , which are constrained to point along the local easy-axis directions and can thus be described by the Ising pseudospin variables, σi=±1. The Hamiltonian comprises an exchange term of strength J between nearest-neighbour spins 〈i, j〉, and long-range dipolar interactions of characteristic strength D=(μ0/4π)μ2/ between all pairs of spins, where μ≈10 μB is the magnitude of the Dy3+ spin and rnn is the nearest-neighbour distance of the lattice. The Hamiltonian is thus given by
where rij is the vector of length rij connecting spins i and j. We use D=1.28 K as calculated from experimentally determined Dy-Dy distances, and J=−3.72 K from Dy2Ti2O7 (ref. 27), which has a similar Dy environment to Dy3Mg2Sb3O14 (ref. 22) (Supplementary Fig. 3). We treat the long-range dipolar interactions using Ewald summation58,59 with tinfoil boundary conditions at infinity. In simulations including site disorder, non-magnetic ions are simulated by setting the corresponding σi to zero. Our unit cell comprises three stacked kagome layers, each layer made from four kagome triangles. The whole system comprises N=7776 spins in total, commensurate with the possible × spin-ordered state found in 2D (ref. 8). We use both single-spin flip and loop dynamics58,60, with Metropolis weights. Loop dynamics are necessary to ensure ergodicity at low temperatures and explore possible long-range spin-ordered states. We use the short loop algorithm58,60. One Monte Carlo sweep is defined as N single spin-flip attempts, followed by the proposal of loop moves until the cumulative number of proposed spin-flips (in the loops) is at least N. We use an annealing protocol, initializing the system at high temperature with ∼104N single spin-flip attempts, then decrease the temperature incrementally. After each temperature decrement, the system is updated with ∼103 Monte Carlo sweeps to ensure equilibration before collecting data every ∼10 Monte Carlo sweeps. Powder-averaged magnetic neutron-scattering patterns calculated from Monte Carlo are shown in Supplementary Fig. 9.
The underlying research materials can be accessed at the following location: http://dx.doi.org/10.17863/CAM.4902.
How to cite this article: Paddison, J. A. M. et al. Emergent order in the kagome Ising magnet Dy3Mg2Sb3O14. Nat. Commun. 7, 13842 doi: 10.1038/ncomms13842 (2016).
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
de Vries, M. A. et al. Scale-free antiferromagnetic fluctuations in the s=1/2 kagome antiferromagnet herbertsmithite. Phys. Rev. Lett. 103, 237201 (2009).
Han, T.-H. et al. Fractionalized excitations in the spin-liquid state of a kagome-lattice antiferromagnet. Nature 492, 406–410 (2012).
Fåk, B. et al. Kapellasite: A kagome quantum spin liquid with competing interactions. Phys. Rev. Lett. 109, 037208 (2012).
Mendels, P. & Bert, F. Quantum kagome frustrated antiferromagnets: One route to quantum spin liquids. C. R. Phys. 17, 455–470 (2016).
Zhou, H. D. et al. Partial field-induced magnetic order in the spin-liquid kagomé Nd3Ga5SiO14 . Phys. Rev. Lett. 99, 236401 (2007).
Zorko, A., Bert, F., Mendels, P., Marty, K. & Bordet, P. Ground state of the easy-axis rare-earth kagome langasite Pr3Ga5SiO14 . Phys. Rev. Lett. 104, 057202 (2010).
Cairns, A. B. et al. Encoding complexity within supramolecular analogues of frustrated magnets. Nat. Chem. 8, 442–447 (2016).
Chern, G.-W., Mellado, P. & Tchernyshyov, O. Two-stage ordering of spins in dipolar spin ice on the kagome lattice. Phys. Rev. Lett. 106, 207202 (2011).
Wills, A. S., Ballou, R. & Lacroix, C. Model of localized highly frustrated ferromagnetism: The kagomé spin ice. Phys. Rev. B 66, 144407 (2002).
Bramwell, S. T. & Gingras, M. J. Spin ice state in frustrated magnetic pyrochlore materials. Science 294, 1495–1501 (2001).
Castelnovo, C., Moessner, R. & Sondhi, S. L. Magnetic monopoles in spin ice. Nature 451, 42–45 (2008).
Möller, G. & Moessner, R. Magnetic multipole analysis of kagome and artificial spin-ice dipolar arrays. Phys. Rev. B 80, 140409 (2009).
Brooks-Bartlett, M. E., Banks, S. T., Jaubert, L. D. C., Harman-Clarke, A. & Holdsworth, P. C. W. Magnetic-moment fragmentation and monopole crystallization. Phys. Rev. X 4, 011007 (2014).
Canals, B. et al. Fragmentation of magnetism in artificial kagome dipolar spin ice. Nat. Commun. 7, 11446 (2016).
Fennell, T., Bramwell, S. T., McMorrow, D. F., Manuel, P. & Wildes, A. R. Pinch points and Kasteleyn transitions in kagome ice. Nat. Phys. 3, 566–572 (2007).
Matsuhira, K., Hiroi, Z., Tayama, T., Takagi, S. & Sakakibara, T. A new macroscopically degenerate ground state in the spin ice compound Dy2Ti2O7 under a magnetic field. J. Phys.: Condens. Matter 14, L559 (2002).
Mengotti, E. et al. Real-space observation of emergent magnetic monopoles and associated Dirac strings in artificial kagome spin ice. Nat. Phys. 7, 68–74 (2011).
Zhang, S. et al. Crystallites of magnetic charges in artificial spin ice. Nature 500, 553–557 (2013).
Anghinolfi, L. et al. Thermodynamic phase transitions in a frustrated magnetic metamaterial. Nat. Commun. 6, 8278 (2015).
Dun, Z. L. et al. Magnetic ground states of the rare-earth tripod kagome lattice Mg2RE3Sb3O14 (RE=Gd,Dy,Er). Phys. Rev. Lett. 116, 157201 (2016).
Bramwell, S. T., Field, M. N., Harris, M. J. & Parkin, I. P. Bulk magnetization of the heavy rare earth titanate pyrochlores - a series of model frustrated magnets. J. Phys.: Condens. Matter 12, 483 (2000).
Farmer, J. M. et al. Structural and crystal chemical properties of rare-earth titanate pyrochlores. J. Alloys Comp. 605, 63–70 (2014).
Pomaranski, D. et al. Absence of Pauling’s residual entropy in thermally equilibrated Dy2Ti2O7 . Nat. Phys. 9, 353–356 (2013).
Hallas, A. M. et al. Statics and dynamics of the highly correlated spin ice Ho2Ge2O7 . Phys. Rev. B 86, 134431 (2012).
McGreevy, R. L. & Pusztai, L. Reverse Monte Carlo simulation: A new technique for the determination of disordered structures. Mol. Simul. 1, 359–367 (1988).
Paddison, J. A. M. & Goodwin, A. L. Empirical magnetic structure solution of frustrated spin systems. Phys. Rev. Lett. 108, 017204 (2012).
den Hertog, B. C. & Gingras, M. J. P. Dipolar interactions and origin of spin ice in Ising pyrochlore magnets. Phys. Rev. Lett. 84, 3430–3433 (2000).
Chioar, I. A., Rougemaille, N. & Canals, B. Ground-state candidate for the classical dipolar kagome Ising antiferromagnet. Phys. Rev. B 93, 214410 (2016).
Fennell, T. et al. Magnetic coulomb phase in the spin ice Ho2Ti2O7 . Science 326, 415–417 (2009).
Sakakibara, T., Tayama, T., Hiroi, Z., Matsuhira, K. & Takagi, S. Observation of a liquid-gas-type transition in the pyrochlore spin ice compound Dy2Ti2O7 in a magnetic field. Phys. Rev. Lett. 90, 207205 (2003).
Hamp, J., Chandran, A., Moessner, R. & Castelnovo, C. Emergent Coulombic criticality and Kibble-Zurek scaling in a topological magnet. Phys. Rev. B 92, 075142 (2015).
Petit, S. et al. Observation of magnetic fragmentation in spin ice. Nat. Phys. 12, 746–750 (2016).
Champion, J. D. M. et al. Order in the heisenberg pyrochlore: the magnetic structure of Gd2Ti2O7 . Phys. Rev. B 64, 140407 (2001).
Stewart, J. R., Ehlers, G., Wills, A. S., Bramwell, S. T. & Gardner, J. S. Phase transitions, partial disorder and multi-k structures in Gd2Ti2O7 . J. Phys.: Condens. Matter 16, L321 (2004).
Zhou, H. D. et al. Intrinsic spin-disordered ground state of the Ising garnet Ho3Ga5O12 . Phys. Rev. B 78, 140406 (2008).
Snyder, J. et al. Low-temperature spin freezing in the Dy2Ti2O7 spin ice. Phys. Rev. B 69, 064414 (2004).
Matsuhira, K. et al. Spin dynamics at very low temperature in spin ice Dy2Ti2O7 . J. Phys. Soc. Jpn. 80, 123711 (2011).
Sanders, M. B., Krizan, J. W. & Cava, R. J. RE3Sb3Zn2O14 (RE=La, Pr, Nd, Sm, Eu, Gd): a new family of pyrochlore derivatives with rare earth ions on a 2D kagome lattice. J. Mater. Chem. C 4, 541–550 (2016).
Sanders, M. B., Baroudi, K. M., Krizan, J. W., Mukadam, O. A. & Cava, R. J. Synthesis, crystal structure, and magnetic properties of novel 2D kagome materials RE3Sb3Mg2O14 (RE=La, Pr, Sm, Eu, Tb, Ho): comparison to RE3Sb3Zn2O14 family. Phys. Stat. Solidi B 253, 2056–2065 (2016).
Scheie, A. et al. Effective spin-1/2 scalar chiral order on kagome lattices in Nd3Sb3Mg2O14 . Phys. Rev. B 93, 180407 (2016).
Fennell, T., Bramwell, S. T. & Green, M. A. Structural and magnetic characterization of Ho3SbO7 and Dy3SbO7 . Can. J. Phys. 79, 1415–1419 (2001).
Hannon, A. C. Results on disordered materials from the GEneral Materials diffractometer, GEM, at ISIS. Nucl. Instr. Meth. Phys. Res. A 551, 88–107 (2005).
Copley, J. & Cook, J. The Disk Chopper Spectrometer at NIST: a new instrument for quasielastic neutron scattering studies. Chem. Phys. 292, 477–485 (2003).
Azuah, R. T. et al. DAVE: A comprehensive software suite for the reduction, visualization, and analysis of low energy neutron spectroscopic data. J. Res. Natl. Inst. Stan. Technol. 114, 341 (2009).
Rodríguez-Carvajal, J. Recent advances in magnetic structure determination by neutron powder diffraction. Physica B 192, 55–69 (1993).
Henelius, P. et al. Refrustration and competing orders in the prototypical Dy2Ti2O7 spin ice material. Phys. Rev. B 93, 024402 (2016).
Filippi, J., Lasjaunias, J., Ravex, A., Tchéou, F. & Rossat-Mignod, J. Specific heat of dysprosium gallium garnet between 37 mK and 2 K. Solid State Commun. 23, 613–616 (1977).
Wills, A. S. Magnetic structures and their determination using group theory. J. Phys. IV France 11, 133–158 (2001).
Wills, A. S. A new protocol for the determination of magnetic structures using simulated annealing and representational analysis (SARAh). Physica B 276-278, 680–681 (2000).
Campbell, B. J., Stokes, H. T., Tanner, D. E. & Hatch, D. M. ISODISPLACE: a web-based tool for exploring structural distortions. J. Appl. Crystallogr. 39, 607–614 (2006).
Kovalev, O. V. Representations of the Crystallographic Space Groups Gordon and Breach Science Publishers (1993).
Siqueira, K. P. F. et al. Crystal structure of fluorite-related Ln3SbO7 (Ln=La-Dy) ceramics studied by synchrotron X-ray diffraction and Raman scattering. J. Solid State Chem. 203, 326–332 (2013).
Paddison, J. A. M., Stewart, J. R. & Goodwin, A. L. Spinvert: a program for refinement of paramagnetic diffuse scattering data. J. Phys.: Condens. Matter 25, 454220 (2013).
Brown, P. J. International Tables for Crystallography vol. C, 454–460Kluwer Academic Publishers (2004).
Frey, F. Diffuse scattering from disordered crystals. Acta Crystallogr. B 51, 592–603 (1995).
Mellergård, A. & McGreevy, R. L. Reverse Monte Carlo modelling of neutron powder diffraction data. Acta Crystallogr. A 55, 783–789 (1999).
Blech, I. A. & Averbach, B. L. Spin correlations in MnO. Physics 1, 31–44 (1964).
Melko, R. G. & Gingras, M. J. P. Monte Carlo studies of the dipolar spin ice model. J. Phys.: Condens. Matter 16, R1277 (2004).
de Leeuw, S. W., Perram, J. W. & Smith, E. R. Simulation of electrostatic systems in periodic boundary conditions. I. Lattice sums and dielectric constants. Proc. R. Soc. London A 373, 27–56 (1980).
Melko, R. G., den Hertog, B. C. & Gingras, M. J. P. Long-range order at low temperatures in dipolar spin ice. Phys. Rev. Lett. 87, 067203 (2001).
Work at Cambridge was supported through the Winton Programme for the Physics of Sustainability. The work of J.A.M.P., X.B. and M.M. and facilities at Georgia Tech were supported by the College of Sciences through M.M. start-up funds. J.A.M.P. gratefully acknowledges Churchill College, Cambridge for the provision of a Junior Research Fellowship. H.S.O. acknowledges a Teaching Scholarship (Overseas) from the Ministry of Education, Singapore. J.O.H. is grateful to the Engineering and Physical Sciences Research Council (EPSRC) for funding. C.C. was supported by EPSRC Grant No. EP/G049394/1, and the EPSRC NetworkPlus on ‘Emergence and Physics far from Equilibrium’. Experiments at the ISIS Pulsed Neutron and Muon Source were supported by a beamtime allocation from the Science and Technology Facilities Council. This work utilized facilities at the NIST Center for Neutron Research. Monte Carlo simulations were performed using the Darwin Supercomputer of the University of Cambridge High Performance Computing Service (http://www.hpc.cam.ac.uk/) and the ARCHER UK National Supercomputing Service (http://www.archer.ac.uk/, for which access was provided by an ARCHER Instant Access scheme). We thank G.-W. Chern, J. Goff, A. L. Goodwin, G. Lonzarich, G. Moller, D. Prabhakaran, J. R. Stewart and A. Zangwill for valuable discussions, and M. Kwasigroch for preliminary theoretical work.
The authors declare no competing financial interests.
About this article
Cite this article
Paddison, J., Ong, H., Hamp, J. et al. Emergent order in the kagome Ising magnet Dy3Mg2Sb3O14. Nat Commun 7, 13842 (2016). https://doi.org/10.1038/ncomms13842
This article is cited by
npj Quantum Materials (2021)
Nature Communications (2021)
Journal of Low Temperature Physics (2020)
Nature Communications (2018)
Nature Communications (2017)